sheet metal forming220.127.116.11/pics_upload/sheet metal forming2.pdf · sheet metal forming •...
Post on 13-May-2020
Embed Size (px)
Sheet Metal Forming
Sheet Metal Forming
• For products with versatile shapes and lightweight • Dates to 5000 B.C. • Products include metal desks, file cabinets, appliances, car bodies, beverage cans
• Common materials: lowcarbon steel, aluminum or titanium
• First take sheet plate and cut into pieces by shearing, slitting, cutting, or sawing or produce from coil
• Then form into shapes by punching, blanking, stamping, embossing, bending, forming, deep drawing, and a variety of other processes
Sheet Metal Characteristics TABLE 16.2 Characteristic Importance Elongation Determines the capability of the sheet metal to stretch without necking and failure; high
strainhardening exponent (n)and strainrate sensitivity exponent (m)desirable. Yieldpoint elongation Observed with mildsteel sheets; also called Lueder’s bands and stretcher strains; causes
flamelike depressions on the sheet surfaces; can be eliminated by temper rolling, but sheet must be formed within a certain time after rolling.
Anisotropy (planar) Exhibits different behavior in different planar directions; present in coldrolled sheets because of preferred orientation or mechanical fibering; causes earing in drawing; can be reduced or eliminated by annealing but at lowered strength.
Anisotropy (normal) Determines thinning behavior of sheet metals during stretching; important in deep drawing operations.
Grain size Determines surface roughness on stretched sheet metal; the coarser the grain, the rougher the appearance (orange peel); also affects material strength.
Residual stresses Caused by nonuniform deformation during forming; causes part distortion when sectioned and can lead to stresscorrosion cracking; reduced or eliminated by stress relieving.
Springback Caused by elastic recovery of the plastically deformed sheet after unloading; causes distortion of part and loss of dimensional accuracy; can be controlled by techniques such as overbending and bottoming of the punch.
Wrinkling Caused by compressive stresses in the plane of the sheet; can be objectionable or can be useful in imparting stiffness to parts; can be controlled by proper tool and die design.
Quality of sheared edges Depends on process used; edges can be rough, not square, and contain cracks, residual stresses, and a workhardened layer, which are all detrimental to the formability of the sheet; quality can be improved by control of clearance, tool and die design, fine blanking, shaving, and lubrication.
Surface condition of sheet Depends on rolling practice; important in sheet forming as it can cause tearing and poor surface quality; see also Section 13.3.
• Formability is the ability of sheet metal to undergo shape change without failure by necking or tearing
• Cupping (Swift or Ericson) tests give some idea of formability
(a) Yieldpoint elongation in a sheetmetal specimen. (b) Lueder's bands in a lowcarbon steel sheet. Source: Courtesy of Caterpillar Inc. (c) Stretcher strains at the bottom of a steel can for household products.
(a) (b) (c)
FormingLimit Diagrams (FLD)
• Sheet metal is marked with small circles, stretched over a punch, and deformation is observed in failure areas
• FLD shows boundary between safe and failure zones
(a) Strains in deformed circular grid patterns. (b) Forminglimit diagrams (FLD) for various sheet metals. Although the major strain is always positive (stretching), the minor strain may be either positive or negative. In the lower left of the diagram, R is the normal anisotropy of the sheet, as described in Section 16.9.2. Source: S. S. Hecker and A. K. Ghosh.
(a) Schematic illustration of shearing with a punch and die, indicating some of the process variables. Characteristic features of (b) a punched hole and (c) the slug. Note that the scales of the two figures are different.
• A blank is a properly sized piece of sheet metal removed from a much larger sheet or coil by shearing
• Shearing is cutting by subjecting a workpiece to shear stresses
• Shearing starts with small cracks at points A, B, C, D which eventually grow and meet
• Rough fracture surfaces and smooth burnished surfaces result
• Shear angles or beveled edges often used on shearing dies
• Clearance, c, between the punch and die typically between 2% and 10% of sheet metal thickness
• As clearance increases, sheared edge becomes rougher and zone of deformation becomes larger – clearances are smaller for softer metals, thinner sheets, or larger holes
• Ratio of burnished to rough edges increases with: increasing ductility, decreasing clearance and thickness
• Faster punch speeds cause narrower sheared zones and less burr formation
• Burr height increases with increasing clearance, ductility, or dull tools
• Maximum Punch Force, F = 0.7 T L (UTS) (product of thickness, sheared edge perimeter, and UTS)
• Punching – sheared slug is discarded • Blanking – slug is workpiece, surrounding area discarded • Die cutting includes perforating (many holes), parting (separating into multiple pieces), notching (removing pieces from the edges), and lancing (leaving a tab)
• Fine blanking with 1% clearances produces very smooth and squared off edges (a) (b)
(a) Comparison of sheared edges produced by conventional (left) and by fineblanking (right) techniques. (b) Schematic illustration of one setup for fine blanking. Source: Feintool U.S. Operations.
• Slitting – cutting off with 2 circular blades (can opener) • Steel rules – a die for shearing soft metals, paper, leather, and rubber into specific shapes (cookie cutter)
• Nibbling – reciprocating die for successive, overlapping holes that shears intricate, flexible shapes
• Shaving – trims excess material to clean sheared edges • Compound and progressive dies perform several operations
Slitting with rotary knives. Shaving and
Other Methods of Cutting Sheet Metal
• Band saw – metal material removal process that produces chips as in other machining
• Flame cutting – especially for thick steel plates, as in shipbuilding
• Laserbeam cutting – newer process used with computer controlled equipment
• Plasma cutting – high energy plasma formed by electric arc between tool and work material
• Friction sawing – disk or blade that rubs against sheet or plate at high speeds
• Waterjet cutting – for metallic and nonmetallic workpieces
Mechanical Stamp Press
Sequential Process Steps
Progressive Die Work
• Design parts with straight parallel edges and “jigsaw” ends minimizes scrap and can be produced on simplest cutoff die
Cut Off Operation
Part Off Operation
• Design parts with straight parallel edges reduces edge scrap and requires simpler partoff die
Hole Punching Die
Blank and Punch Die
Processing Limits –minimum hole diameters
Critical Dimensions in Design of Sheet Metal Blank
* All dimensions > 2 x gage thickness
Feature Position Limits
* Dimension > 4 x gage thickness
• Scrap metal can be as high as 30% • Computer aided design and planning can minimize scrap • Tailorwelded blanks are multiple pieces of flat sheet butt welded together and simultaneously stamped
Production of an outer side panel of a car body, by laser buttwelding and stamping. Source: After M. Geiger and T. Nakagawa.
Reducing Waste Material